Chapter 2Industrial Waste Aggregates2.1 IntroductionThe aggregates typically account for 70–80 % of the concrete volume and play asubstantial role in different concrete properties such as workability, strength,dimensional stability and durability. Conventional concrete consists of sand as ﬁneaggregate and gravel, limestone or granite in various sizes and shapes as coarseaggregate. There is a growing interest in using waste materials as alternativeaggregate materials and signiﬁcant research is made on the use of many differentmaterials as aggregate substitutes such as coal ash, blast furnace slag, ﬁbre glasswaste materials, waste plastics, rubber waste, sintered sludge pellets and others.The consumption of waste materials can be increased manifold if these are used asaggregate into cement mortar and concrete. This type of use of a waste materialcan solve problems of lack of aggregate in various construction sites and reduceenvironmental problems related to aggregate mining and waste disposal. The useof waste aggregates can also reduce the cost of the concrete production. As theaggregates can signiﬁcantly control the properties of concrete, the properties of theaggregates have a great importance. Therefore a thorough evaluation is necessarybefore using any waste material as aggregate in concrete. Signiﬁcant work hasbeen done on the use of several types of waste materials as an aggregate inpreparation of cement mortar and concrete. In this section, various properties ofsome waste materials used as aggregate will be presented.2.2 Types of Industrial Waste AggregatesThe properties of waste aggregates that will be highlighted in this section are:1. Plastics wastes; 2. Coal ash; 3. Rubber tyre; 4. Slags; 5. Waste from food andagricultural industries; 6. Pulp and paper mill waste; 7. Leather waste; 8. Industrialsludge; 9. Mining industry waste.J. de Brito and N. Saikia, Recycled Aggregate in Concrete, 23Green Energy and Technology, DOI: 10.1007/978-1-4471-4540-0_2,Ó Springer-Verlag London 2013
24 2 Industrial Waste Aggregates Depending on their generation, wastes can be separated into two types: thosethat directly result from industry as industrial by-products and those that can benamed recycled wastes. The ﬁrst type includes coal ash, various slags from metalindustries, industrial sludge, waste from industries like pulp and paper mills, minetailings, food and agriculture, and leather. The second type includes differentplastic and rubber wastes. A broad classiﬁcation of industrial waste aggregate can be made depending onthe chemical nature of wastes. Some waste aggregates come from production anduse of organic materials. Plastics, rubber, leather and some food industries wastesare organic wastes. On the other hand, industrial slags, mining wastes, coalindustry wastes and others are inorganic wastes. Glass reinforced plastics andsome industrial sludge may contain both organic and inorganic materials. Another classiﬁcation of industrial waste aggregate can be done depending onthe weight of waste aggregates. Some aggregates are lightweight by nature.Plastics, rubber, most food and agricultural industries wastes and coal bottom ashare of this kind. On the other hand, most of the industrial slags are heavier thanconventional aggregates.2.3 Coal Ash as an Aggregate in ConcreteBurning of coal generates two types of waste materials: ﬂy ash and bottom ash.There are two types of bottom ashes, wet bottom boiler slag and dry bottom ashdepending on both the boiler type and its design. Coal ﬂy ash, also known as pulverised fuel ash, is the ﬁnest fraction of theseashes, which are released from combustion chamber and transported by ﬂue gases.Fly ash contains the non-combustible matter in coal along with a small amount ofcarbon that remains from incomplete coal combustion. Fly ash consists mostly ofsilt-sized and clay-sized glassy spheres. When pulverised coal is burned in a drybottom boiler about 80 per cent of the unburned material or ash is entrained in theﬂue gas and is captured and recovered as ﬂy ash. The remaining 20 % ash that iscollected from the bottom of furnaces is called coal bottom ash (CBA), which is acoarse, incombustible by-product with a grain size similar to that of ﬁne and coarsesized natural aggregates. Bottom ash is produced as a granular material andremoved from the bottom of dry boilers. Boiler slag, a coarse grained product, is produced from two types of wet bottomboilers, slag-tap and cyclone boilers. The slag-tap boiler burns pulverised coalwhile the cyclone boiler burns crushed coal. Both boiler types have a solid basewith an oriﬁce that can be opened to allow molten ash to ﬂow into a hopper, whichcontains quenching water. When the molten slag comes in contact with thequenching water, the ash fractures instantly, crystallises, and forms pellets. High-pressure water jets wash the boiler slag from the hopper into a sluiceway, whichthen transmits the ash to collection basins for dewatering and further processing.Boiler slag is a coarse, angular, glassy, black material. When pulverised coal is
2.3 Coal Ash as an Aggregate in Concrete 25burned in a slag-tap furnace, as much as 50 % of the ash is retained in the furnaceas boiler slag. In a cyclone furnace, which burns crushed coal, 70–85 % of the ashis retained as boiler slag. Properties of coal ash depend on coal type, pulverising system, combustionconditions, temperature, type of furnace, minerals in coals and milling system.Though a signiﬁcant number of references are available on the properties and useof ﬂy ash as a mineral addition in normal Portland cement, not much literatureexists on the use of ﬂy ash, coal bottom ash (CBA) and boiler slag as a granularadditive into concrete. Again compared to CBA, very little work has been done onthe use of other two ashes as aggregate in concrete. The properties of these asheswill be discussed separately.2.3.1 Bottom Ash18.104.22.168 Dry Bottom AshSome of physical properties of ash generated from dry bottom boiler (henceforthcalled coal bottom ash, CBA) as aggregate are presented in Table 2.1. Theseproperties depend on the burning efﬁciency, the method by which the CBA isobtained and the type of combustion and thus the physical properties of bottom ashgreatly vary in reported works. The density parameters of CBA are considerablylower than those of natural sand (*2.6 g/cm3) and therefore CBA can be used aslightweight aggregate in concrete. CBA with relatively low density or speciﬁcgravity is often indicative of the presence of porous particles. Bottom ash withrelatively high speciﬁc gravity (above 3.0) may indicate the presence of highamounts of iron. The bottom ash is a porous material and generally has high waterabsorption capacity. However, variation in water absorption capacity in differentCBA is quite large, with a range of 2–32 %. The moisture content of bottom ashused by Andrade et al. (2009) as a ﬁne aggregate in concrete is about 55 %. On theother hand, CBA is more brittle than natural sand and has a greater resemblance tocement clinker (Rogbeck and Knutz 1999). The porosity and void content of CBA are generally higher than in naturalaggregate and thus CBA can accommodate a high amount of water in a concretemix. Therefore there is some difﬁculty in determining the exact water/cement ratioof concrete mixes containing CBA. However, the ability to incorporate highamount of water by CBA can be used as a reservoir of water for future hydration ofcement. This behaviour, commonly known as internal curing is particularly usefulfor high strength concrete, where less water is used to make concrete. In this typeof concrete, the hydration process leads to shortage of water in the cement paste.At this stage, the water content in CBA can promote a supply of water internally tothe concrete for continuous hydration. These hydration products ﬁll the pores ormicro-cracks and improve concrete properties.
26Table 2.1 Physical properties of coal bottom ash reported as aggregate in concreteReference Properties Unit weight, kg/ Speciﬁc gravity/ Water Fineness Moisture Maximum Porosity #Void m3 density, kg/m3 absorption (%) modulus content (%) diameter (mm) content (%)Kou and Poon (2009) 2,190 (SSD) 28.9 (1 h) 1.83Andrade et al. (2007) 1.674 (sp. gr.) 1.55 55Andrade et al. (2007) 1.67 (sp. gr.) 1.60 2.4Bai et al. (2005) 1.50 (SSD, sp. gr.) 30.4 (1 h)Bai et al. (2005) 1.58 32.2 (1 h) 5.0Kim and Lee (2011) 1.77 (OD) 1.87 (SSD) 5.45 (ASTM) 2.36 2.4 10.19aKim and Lee (2011) 1.64 (OD) 1.77 (SSD) 8.14 (ASTM) 13.2 13.34aYuksel et al. 620 (loose) 660 1.39 6.10 (TS) 4.0 (dense)Ghafoori and 2.33 (OD) 2.47 (SSD) 7.0 2.80 Bucholc (1996)Lee et al. (2010) 1,268 1.84 (OD) 1.90 (SSD) 1.59 2 #33.3 2 988 1.98 (OD) 2.00 (SSD) 3.81 8 #50.4 1,040 1.78(OD) 1.90 (SSD) 11 #45.1Park et al. (2009) 1,275 2,410 2.43 13Kou and Poon (2009) 1,270 2,480 2.11 20 aSSD saturated surface-dry; sp. gr. speciﬁc gravity; TS Turkish standard, TS EN-12620; water accessible porosity Industrial Waste Aggregates
2.3 Coal Ash as an Aggregate in Concrete 27Fig. 2.1 Particle size distribution of a CBA and of natural sand a Bai et al. (2005); b Ghafooriand Bucholc (1996) The particle size of CBA also depends on the factors indicated earlier. Inliterature, the use of CBA as ﬁne or coarse aggregate is reported (Table 2.1). TheCBA used in Ghafoori and Bucholc (1996) study was an well-graded ﬁneaggregate with a ﬁneness modulus (FM) of 2.80 (ASTM’s recommendation of FMrange for ﬁne aggregate is 2.3–3.1). Figure 2.1 shows the particle size distributionof two typical CBA used as partial substitution of ﬁne aggregate in concrete. Compared to natural sand aggregate, which is dense, normally smooth in texture,and round in shape. The particles of CBA aggregate are porous and angular in shape.It has rough surface texture, large numbers of micro-pores (circular holes with adiameter in a range of 0.5–5 lm) and internal pores. Some spherical shaped ﬂy ashparticles having a few micrometer diameters can be deposited on the surfaces of CBA(Kim and Lee 2011). The shape and porous structure of CBA makes it necessary touse a high amount of water during preparation of the concrete mix. A typical pore-size distribution curve of bottom ash (presented in Fig. 2.2) indicates that thenanostructure of bottom ash is quite dense (Kim and Lee 2011). The chemical properties of CBA are normally controlled by the properties ofcoal (its origin). Table 2.2 shows oxide composition of some CBA samples. CBAis composed primarily of silica (SiO2), ferric oxide (Fe2O3) and alumina (Al2O3),with smaller quantities of calcium oxide (CaO), potassium oxide (K2O), sodiumoxide (Na2O), magnesium oxide (MgO), titanium oxide (TiO2), phosphorouspentoxide (P2O5) and sulphur trioxide (SO3). The minerals identiﬁed in different CBA used as aggregate in concrete arepresented in Table 2.2. Figure 2.3 shows the X-ray diffraction (XRD) pattern oftypical low calcium CBA. The major minerals found in CBA are quartz, mulliteand a non-crystalline glassy phase. In some CBA, iron containing minerals likehematite and magnetite may also be present. The fused and glassy texture of CBAnormally would make an ideal substitute for the aggregate fraction of concrete. Unlike its companion—pulverised fuel ash (PFA) or coal ﬂy ash, CBA usuallyhas low pozzolanicity, which makes it unsuitable to be used as a mineral additionin cement. It may contain higher concentrations of unburned carbon. Some powerplants recover coal mill rejects with bottom ash and therefore CBA may containpyrites that come from mill rejects, which can cause expansion in concrete.
28 2 Industrial Waste AggregatesFig. 2.2 Pore sizedistribution of bottom ash(Kim and Lee 2011)22.214.171.124 Boiler Slag or Wet Bottom AshBoiler slag is a vitriﬁed material, which is a very durable and environmentallystable form that permanently immobilises its chemical constituents into the glassyamorphous structure. Boiler slag is made of porous, glassy, angular, uniform sizedsmooth granular particles. The quenched slag becomes somewhat vesicular orporous if gases are trapped in the slag. Boiler slag generated from burning oflignite or sub-bituminous coal tends to be more porous than that of bituminouscoals (Lovell and Te-Chih 1992). The boiler slag primarily comprises particles, which can be regarded as single-sized coarse to ﬁne sand with 90–100 % passing a 4.75 mm mesh sieve, 40–60 %passing a 2.0 mm mesh, 10 % or less passing a 0.42 mm mesh and 5 % or lesspassing a 0.075 mm mesh (Majizadeh et al. 1979). Boiler slag is black in colour,hard, and durable with a resistance to surface wear. Boiler slag typically contains 40–60 % SiO2, 18–38 % Al2O3, 2–7 % Fe2O3,1–4 % CaO, 0.5–3.0 % MgO and 0.5–2.0 % TiO2. The chemical composition ofboiler slag is also governed by the coal source. Boiler slag exhibits less abrasion andsoundness loss than bottom ash as a result of its glassy surface texture and lowerporosity. The predominate minerals present in boiler slags are mullite, quartz, cal-cium silicate and quicklime. The speciﬁc gravity of boiler slag usually ranges from2.3 to 2.9. The dry unit weight of boiler slag usually ranges from 960 to 1,440 kg/m3.Occasionally, the dry unit weight of boiler slag may reach 1,760 kg/m3. Deleterious materials, such as soluble sulphates or coal pyrites, should beremoved from the bottom ash and boiler slag before attempting to use thesematerials as an aggregate. Pyrites can be removed from the coal before it is burnedusing sink-ﬂoat techniques, or from the bottom ash or boiler slag using magneticseparation. Due to salt content (soluble chlorides and sulphates) and low pH andelectrical resistivity, bottom ash and boiler slag may be potentially corrosive andtherefore evaluation of the corrosive nature of the bottom ash being used should beinvestigated. Corrosivity indicator tests normally used to evaluate bottom ash arepH, electrical resistivity, soluble chloride content and soluble sulphate content.
Table 2.2 Chemical and physical characteristics of bottom ashContent Andrade et al. Bai et al. Cheriaf et al. Kou and Lee et al. Ozkan et al. Kurama et al. (2009) Park et al. Ghafoori and(%) (2007) (2005) (1999) Poon (2009) (2010) (2007) (2009) Bucholc (1996)Country Brazil UK French China SKorea Turkey Turkey SKorea USAOrigin nr nr Low-grade coal nr nr nr nr nr LigniteChemical analysisSiO2 50.46 61.80 56.00 60.7 44.2, 48.0 59.53 54.5 47.9 41.70Al2O3 28.35 17.80 26.70 18.3 31.5, 31.3 20.12 15.4 25.94 17.10Fe2O3 10.69 6.97 5.80 6.56 8.87, 8.26 13.08 11.16 4.76 6.63Na2O nr 0.95 0.20 0.89 nr – nr 1.38 1.38K2 O 3.81 2.00 2.60 2.12 4.04, 4.14 0.06 1.34 0.67 0.40CaO 2.07 3.19 0.80 3.25 2.00, 1.41 2.02 4.69 2.48 22.50TiO2 1.57 0.88 1.30 0.95 2.38, 2.29 nr nr 0.86 nrSO3 0.34 0.79 0.1 (as S) 0.82 1.3, 1.2 Trace 1.30 1.03 0.42 2.3 Coal Ash as an Aggregate in ConcreteZrO2 0.18 nr nr nr nr nr nr nr nrV2O5 0.09 nr nr nr 0.07, 0.09 nr nr nr nrMnO 0.07 nr nr nr 0.07, 0.06 nr nr nr nrZnO 0.03 nr nr nr nr nr nr nr nrY2O3 0.03 nr nr nr nr nr nr nr nrSrO 0.03 nr nr nr nr nr nr nr nrMgO nr 1.34 0.60 1.28 2.6, 2.0 3.20 4.26 1.10 4.91Cr2O3 nr nr nr nr 0.03, 0.05 nr nr nr nrP2O5 nr 0.20 nr nr 0.3, 0.33 nr nr nr nrOthers nr 0.49 nr 1.00 0.32, 0.40 nr nr nr 3.83Cl nr nr nr nr 2.32, 0.47 nr nr 0.18 nrLoss on ignition 2.30 3.61 4.60 4.13 nr 9.81 8.90 3.631.13Mineralsnr Quartz, mullite, nr Mullite, quartz, nr nr nr Quartz, magnetite, nr nr glassy phase glassy phase hematite, glassy phase 29nr not reported
30 2 Industrial Waste AggregatesFig. 2.3 The X-raydiffraction pattern oftypical low calcium CBA(Cheriaf et al. 1999)126.96.36.199 Fly AshThe use of ﬂy ash (FA) as partial replacement of normal Portland cement in concreteis very common nowadays and around 15–25 % of cement is generally replaced byFA in normal structural concrete mixes. However, the overall percentage utilisationremains very low in many countries, and most of the ﬂy ash is dumped at landﬁlls(Siddique 2003a, b; Ravina 1997). Much higher quantities of FA can be used inconcrete if ﬂy ash can partially replace the ﬁne sand fraction in concrete mix. Thisreplacement can be made by low quality ﬂy ash too, which has low pozzolanicproperties. Although many references are available on the use of ﬂy ash as a sup-plementary cementing material in concrete, the number of available references on theuse of ﬂy ash as partial replacement of ﬁne aggregates is not very large. American Society for Testing and Materials (ASTM) C618-03 (Standardspeciﬁcation for coal ﬂy ash and raw or calcinated natural pozzolan for use inconcrete), classiﬁes ﬂy ash into two categories—Class F (low calcium) and ClassC (high calcium) ﬂy ash. Combustion of bituminous or anthracite coal normallyproduces Class F (low calcium) ﬂy ash and combustion of lignite or sub-bitumi-nous coal normally produces Class C (high calcium) ﬂy ash. The chemical composition of ﬂy ash used as aggregate in concrete is presentedin Table 2.3. The chemical composition of ﬂy ash depends on the type of coal.More references are available on the use of low calcium ﬂy ash as a replacement ofﬁne aggregate in concrete than high calcium ﬂy ash. High calcium ﬂy ash containslarge amounts of free lime and sulphite than that of low calcium ﬂy ash. Due to thepresence of undesirable chemical components in high calcium ﬂy ash, the use ofthis material is much limited compared to low calcium ﬂy ash. The mineralogical composition of ﬂy ash is very complex. Mineralogically, ﬂyashes are a heterogeneous mixture of mineral phases and amorphous glassy phaseswith small amount of unburned carbon. The glassy phase of low calcium ﬂy ash isalumino-silicate type whereas that of high calcium ﬂy ash is a mixture of calciumaluminate and ferrous alumino-silicate (Das and Yudhbir 2006).
2.3 Coal Ash as an Aggregate in Concrete 31Table 2.3 Chemical composition of some ﬂy ashes used as a replacement of sand fraction inconcreteConstituents/ Siddique Maslehuddin Rajamane Pofale and Papadakis Papadakisproperties (2003a , b) et al. (1989) et al. (2007) Deo (2010) (1999) (2000)SiO2 55.3 60.5 59 55.5 53.50 39.21Al2O3 25.7 23.0 nr 31.3 20.40 16.22Fe2O3 5.3 7.5 nr 6.4 8.66 6.58CaO 5.6 2.0 1.02 1.02 3.38 (free: 22.78 0.36) (free: 5.18)MgO 2.1 1.0 0.30 0.21 – –TiO2 1.3 nr 2.70 – –SO3 1.4 0.3 – 0.44 0.63 4.30Na2O 0.4 nr 0.54 (total – – alkalis)K2O 0.6 nr 0.25 – –LOI 1.9 1.4 1.08 0.74 2.20 2.10Moisture 0.3 nr nr Nr – – contentSiO2 ? Al2O3+ 86.3 91 – 93.2 82.16 62.01 Fe2O3 Depending on the ﬂy ash type, the mineral matter present in ﬂy ash varies sig-niﬁcantly. More than 188 minerals have been identiﬁed in ﬂy ash, most of them traceminerals. High calcium ﬂy ash contains large amounts of calcium-bearing mineralslike lime, anhydrite, gypsum, tricalcium aluminate, alite, gehlenite, akermanite,portlandite and larnite. Some other minerals like quartz, hematite and magnetite arealso present in high calcium ﬂy ash. On the other hand, low calcium ﬂy ash mainlycontains quartz, mullite, hematite, magnetite and small amounts of calcite. Silicon and aluminium are mainly present in a glassy phase, with small amountsof quartz and mullite included. Iron appears partly as oxides (magnetite andhematite), with the rest in a glassy phase. The speciﬁc gravity of ﬂy ash may vary from 1.3 to 4.8 (Joshi and Lohtia 1997).FA mainly consists of clay and silt-sized particles (particle diameter 45 micro-meter), which are generally spherical in shape. There is a wide variation in theparticle size distribution of ﬂy ashes irrespective of the type of ﬂy ash. The particlesize distribution of ﬂy ash mainly depends upon the initial grinding of the coal andthe efﬁciency of the thermal power plant and even ﬂuctuations in power generation(Lee et al. 2010). The shape of the FA may vary depending on the various physicaland chemical factors. The glassy phase is mainly spherical in shape. However,large sized or irregular shaped particles can also be formed from the fusion ofsmaller fragments and incomplete melting. The colour of coal ash depends on itschemical and mineral constituents. High lime containing FA is normally tan andlight in colour. Iron containing FA is brownish in colour. The dark grey to blackcolour of FA indicates the presence of a high amount of unburned carbon.
32 2 Industrial Waste Aggregates2.4 Industrial SlagSlag is a partially vitreous by-product of smelting ore due to separating of themetal fraction from the worthless fraction. It can be considered a mixture of metaloxides; however, slags can contain metal sulphides and metal atoms in theelemental form.2.4.1 Ferrous SlagFerrous slag is produced during the production of iron using blast furnace (blastfurnace slag) as well as in the separation of the molten steel from impurities insteel-making furnaces (steel slag) (Fig. 2.4).188.8.131.52 Steel SlagSteel slag is produced during the separation of molten steel from impurities in steelfurnaces. The slag occurs as a molten liquid and is a complex solution of silicatesand oxides that solidiﬁes upon cooling. There are several different types of steelslag produced during the steel-making process out of which basic oxygen furnacesteel slag (BOF slag), electric arc furnace slag (EAF-slag) and ladle furnace slag(LDF-slag) or reﬁning slag are important. An electric arc furnace produces steel by melting recycled steel scrap, usingheat generated by an arc, created by a large electric current. The slag is formedthrough the addition of lime, which is designed to remove impurities from withinthe steel. Slag has a lower density than steel and therefore ﬂoats on top of themolten bath of steel. In the basic oxygen process, hot liquid blast furnace metal, scrap and ﬂuxes,which consist of lime (CaO) and dolomitic lime (CaO.MgO), are charged into thefurnace. The oxygen, injected into the furnace, combines with and removes theimpurities in the charge. These impurities consist of carbon as gaseous carbonmonoxide, and silicon, manganese, phosphorus and some iron as liquid oxides,which combine with lime and dolomitic lime to form the BOF steel slag. After being tapped from the furnace, molten steel is transferred in a ladle forfurther reﬁning to remove additional impurities still contained within the steel.This operation is called ladle reﬁning because it is completed within the transferladle. During ladle reﬁning, additional steel slags are generated by again addingﬂuxes to the ladle to melt. Steel mill scale is produced during processing of iron in steel mills. During theprocessing of steel in steel mill, iron oxides, known as mill scale are formed on thesurface of the metal during the continuous casting, reheating and hot rolling operations.The steel mill scale is removed by water sprays. The steel mill scale is somewhatsimilar to steel slag and therefore, like steel slag, it can be used in concrete production.
2.4 Industrial Slag 33Fig. 2.4 Flowchart of production of ferrous slag (courtesy Nippon Slag Association) The use of steel slag in the preparation of blended cement, or cement clinker,and as aggregate or hydraulic binder in road construction has been proposed byseveral authors for a long time (Mahieux et al. 2009; Monshi and Asgarani 1999;Shi and Qian 2000). However, not much is reported on the use of steel slag asaggregate in preparation of cement mortar and concrete. Compared to the use of
34 2 Industrial Waste AggregatesBOF-slag as aggregate in concrete, more references are available on EAF-slag. Onthe other hand, LDF-slag is mainly used as a mineral admixture in cement due toits particle size and possibly its mineralogy. Steel slag is a crushed product having hard, dense, angular and roughly cubicalparticles (National Slag Association 2011). The EAF-slag used by Al-Negheimishet al. (1997) as a replacement of coarse aggregate in concrete was angular shapedwith honeycombed surface texture. The angular shape of steel slag aggregate canhelp to develop very strong interlocking properties. The Flakiness Index (FI) of thesteel slag aggregate is markedly lower than those for the dolerite and quartziteaggregates (Anastasiou and Papayianni 2006). The amount of clay lump and fri-able material content in steel slag is considerably lower than in natural aggregates(Almusallam et al. 2004). Anastasiou and Papayianni (2006) evaluated several physical properties ofcrushed steel slag to be used as an aggregate in concrete. The authors concludedthat the evaluated aggregate properties of steel slag are in between the limits of thestandards and in the best categories. Some physical properties of the different typesof steel slags used as aggregate in concrete or asphalt mix and reported by severalresearchers are presented in Table 2.4. Steel slag has higher abrasion resistanceand lower crushing value than natural aggregates. On the other hand, the speciﬁcgravity and water absorption capacity of steel slag are higher than those of con-ventional aggregates. The porosity of a typical steel slag reported by Manso et al.(2004) is 10.5 %. EAF-steel slag aggregates have excellent resistance to frag-mentation (Papayianni and Anastasiou 2010). The surface texture of steel slag is rougher than that of limestone aggregate(Xue et al. 2006; Ahmedzade and Sengoz 2009). The scanning electron micro-graph of EAF-slag indicates the presence of many pores on its surface. Steel slaghas higher bulk density than natural aggregates (Al-Negheimish et al. 1997). An adequate grading of steel slag is necessary to obtain better performancefrom concrete containing steel slag as aggregate (Manso et al. 2006). The particlesize distribution curves of two typical EAF-slags used as coarse and ﬁne aggregatein concrete are presented in Fig. 2.5. Depending on the cooling process, the par-ticle size of steel slag may vary. Air-cooled steel slag consists of large sizedgranules and some powder (Wang et al. 2010). The high content of free lime (free-CaO) and periclase (MgO) is the detrimentalfactor against using various steel slags as aggregate in concrete. The content of freelime (free-CaO) and periclase (MgO) in EAF-slag is considerably lower than inBOF-slag. As steel slag contains expansive materials like CaO and MgO, to beused in concrete slag is generally treated. Ageing or weathering of slag, steam andautoclave curing of slag are generally performed to reduce expansive oxide con-tents (Chen et al. 2007; Faraone et al. 2009; Lun et al. 2008; Pellegrino and Gaddo2009). As the majority of the steel slag contains free CaO and MgO, experimentsare generally performed to evaluate the free CaO and MgO content in the slag andsoundness of steel slag aggregate. Tables 2.5, 2.6 and 2.7 show the chemical compositions of BOF-, LDF- andEAF-slags, respectively. Steel slag is basic in nature (ratio of concentrations of
2.4 Industrial Slag 35Table 2.4 Some physical properties of steel slagProperty Steel Type of Natural Type of natural Reference slag steel slag aggregate aggregateSpeciﬁc gravity 3.51 EAF-slag 2.71 Quartzite Almusallam et al.Los Angeles abrasion (%) 11.6 19.2 (2004).Water absorption (%) 0.85 1.60Speciﬁc gravity 3.64 EAF-slag 2.66 – Al-Negheimish et al. (1997)Water absorption (%) 0.54 1.67Speciﬁc gravity 3.35 EAF-slag Manso et al. (2004)Los Angeles abrasion (%) *20Water absorption (%) 3.29Porosity (%) 10.5 –Speciﬁc gravity 3.02 EAF-slag 2.63 Limestone Ahmedzade andLos Angeles abrasion (%) 20 29 Sengoz (2009)Shape (ﬂat and long) (%) 10 BOF-slag 10 Basalt Xue et al. (2006)LA abrasion (%) 13.1 14.9Crushing value (%) 12.0 12.9Water absorption (%) 1.18 0.70Speciﬁc gravity 3.48 BOF-slag 2.66 River crushed Shen et al. (2009)Water absorption (%) 2.2 1.3 stoneLA abrasion (%) 20.96 23.52Shape (ﬂat and elongated) 5.14 7.55 (%)Roundness index (%) 0.60 0.54CaO ? MgO to SiO2 ? Al2O3 greater than 1) (Tossavainen et al. 2007). The orderof this ratio for LDF-, EAF- and BOF-slags can be arranged as EAF-slag B LDF-slag B BOF-slag. The reactivity and free CaO content of steel slag increases withits increasing basicity (Shi and Qian 2000). Compared to BOF- and LDF-slag,most EAF-slags contain less CaO and MgO in their chemical compositions. Thereare some aggregates reported as steel slags (Maslehuddin et al. 2003; Qasrawiet al. 2009), which contain more than 85 % of Fe2O3 and are therefore completelydifferent from other EAF-slags (Table 2.8). This material can be considered as millscale. The dominant minerals of EAF-slag can be classiﬁed into dicalcium silicate(C2S), merwinite (C3MS2) or kirschsteinite (CFS), depending on the basicity ofsteel slag, of which the basicity of kirschsteinite is the lowest (Qian et al. 2002). Although the concentrations of some toxic metals in steel slag are higher thanthose in normal soil, metals are strongly bound with the slag matrix and thereforeare not readily leached. Therefore, steel slag cannot be considered as ‘‘charac-teristically hazardous’’ material (Proctor et al. 2000). However, in a recent reporthigher leachability values (above the standard limit for inert landﬁll) of Cr and Mofrom EAF-slag were also reported (Tossavainen et al. 2007). As the chemicalcomposition of steel slag is highly variable mineralogical composition of steel slagalso varies. Table 2.9 shows the mineralogical compositions of various types of
36 2 Industrial Waste AggregatesFig. 2.5 Particle sizedistribution curves of twosteel slags (Manso et al.2004)slags as reported by various authors. Different calcium silicates, solid solution ofCaO-FeO-MnO-MgO and free-CaO are the common minerals in steel slag.184.108.40.206 Blast Furnace SlagWhen the blast furnace is tapped to release the molten iron, it ﬂows from thefurnace with molten slag ﬂoating on its upper surface. These two materials areseparated using a weir, the molten iron being channelled to a holding vessel andthe molten slag to a point where it is to be treated further. The ﬁnal form of theblast furnace slag is dependent on the method of cooling. There are four maintypes of blast furnace slag: granulated; air-cooled; expanded and pelletised. Chemically, the blast furnace slag contains mainly silica (30–35 %), calciumoxide (28–35 %), magnesium oxide (1–6 %), and Al2O3/Fe2O3 1.8–2.5 %. Due toits low iron content it can be safely used in the manufacturer of cement. Two typesof blast furnace slag such as air-cooled slag and granulated slag are being gen-erated from the steel plants. The speciﬁc gravity of the slag is approximately 2.90with its bulk density varying in the range of 1,200–1,300 kg/m3. The colour ofgranulated slag is whitish. The air-cooled slag is used as aggregate in road making
Table 2.5 Chemical compositions of BOF-slags 2.4 Industrial SlagAuthor Lun et al. (2008) Xue et al. (2006) Mahieux et al. Tossavainen et al. (2007) Altun and Reddy et al. (2009) Yilmaz (2006) (2002)Country PR China PR China France Sweden Turkey IndiaType Steel slag (from BOF-slag Weathered BOF- BOF-slag BOF-slag BOF-slag BOF) slag S1 S2SiO2 (%) 10.10 13.71 11.8 11.1 18.01 18.87 15.3Al2O3 (%) 1.70 3.80 2.00 1.90 2.61 2.91 1.30Fe and FexOy (%) Fe2O3 = 20.57 FeO = 21.85 Fe2O3 = 22.6 FeO = 10.9 Fe2O3 = 10.7 14.10 11.73 Fe Fe2O3 = 3.24 Fe = 2.30 (total) = 16.2CaO (%) 40.65 45.41 47.5 45.0 37.02 37.94 52.3MnO (%) 0.06 3.27 1.90 3.10 7.52 7.72 0.39MgO (%) 10.88 6.25 6.30 9.60 14.10 14.37 1.1Free lime (%) nr nr nr nr 0.83 0.83 10Basicity: (CaO ? MgO)/ 4.37 2.95 3.90 4.20 2.48 2.40 3.82 (Al2O3 ? SiO2)nr not reported 37
38Table 2.6 Chemical compositions of LDF-slagsAuthor Setien et al. (2009) Tossavainen et al. (2007) Shi and Qian Rodriguez et al. (2000) (2009)Country Spain Sweden PR China SpainType 1 2 3 LDF slag LDF-slag ﬁnes LDF-slagSiO2 (%) 15.0 19.8 12.6 14.2 26.4–26.9 17Al2O3 (%) 12.5 4.3 18.6 22.9 4.3–5.2 11Fe and FexOy (%) Fe2O3 = 2.1 Fe2O3 = 3.3 Fe2O3 = 1.6 Fe2O3 = 1.1 FeO = 0.5 Fe2O3 = 1.0–1.6 nr Fe = 0.4CaO (%) 55.0 57.5 50.5 42.5 56.6–57.0 56MnO (%) 0.36 0.42 0.52 0.2 0.5–1.0MgO (%) 7.5 11.6 11.9 12.6 3.2–4.2 10Free lime (%) 19.0 3.5 9.5 nr nr nrFree MgO (%) 3.0 10.0 8.0 nr nr nr 2Basicity: (CaO ? MgO)/ 2.27 2.87 2.00 1.49 1.93 2.36 (Al2O3 ? SiO2)nr not reported Industrial Waste Aggregates
Table 2.7 Chemical compositions of EAF-slagsAuthor Qian et al. Luxan et al. (2000) Manso et al. (2006) Pellegrino and Gaddo Tossavainen et al. (2007) (2002) (2009)Country Singapore Spain Spain Italy Sweden 2.4 Industrial SlagType Kirschsteinite Black EAF-slag (fusion of Black EAF-slag EAF slag EAF slag based scrap steel) Medium Coarse S1 S2 EAF-slag S1 S2 (contaminated by white slag)SiO2 (%) 19.38 6.04 15.35 15.3 10.1 14.7 32.2 14.1Al2O3 (%) 5.27 14.07 12.21 7.4 5.70 7.20 3.70 6.70Fe and/or FexOy FeO = 30.54 Fe2O3 = 8.49 FeO = 27.41 FeO = 34.36 (%) FeO ? Fe2O3 = 42.5 FeO = 37.2 FeO = 44.8 FeO = 3.30 Fe2O3 = 1.00 FeO = 5.60 Fe2O3 = 20.3 Fe = 0.10 Fe = 0.60CaO (%) 22.48 29.11 24.40 23.9 24.2 29.5 45.5 38.8MnO (%) 1.10 15.58 5.57 4.5 5.10 5.70 2.0 5.0MgO (%) 9.51 3.35 2.91 5.1 1.90 4.60 5.2 3.9Free lime (%) nd nr nr 0.45 nr nr nr nrFree MgO (%) nr nr nr *1.0 nr nr nr nrBasicity: (CaO ? MgO)/ 1.30 1.61 0.99 1.28 (Al2O3 ? SiO2)1.65 1.60 1.41 2.05nd not detected; nr not reported 39
40Table 2.8 Chemical composition of some steel slag described as steel slag or steel making slag and steel mill scaleAuthor Faraone et al. Al-Negheimish et al. Chen et al. (2007) Maslehuddinn et al. Qasrawi et al. Al-Otaibi (2009) (1997) (2003) (2009) (2008)Country Italy Saudi Arabia PR China Saudi Arabia Jordan KuwaitType Steel slag Steel making slag (EAF- Steel slag Steel slag Unprocessed steel Steel mill scale slag) slagSiO2 (%) 13.2 17.43 13.40 1.00 0.80 1.37Al2O3 (%) 6.80 7.85 1.04 nr nr 0.10Fe and/or FexOy (%) FexOy = 9.80 Total Fe = 20.09 FeO = 18.98 FexOy = 89.0 FexOy = 97.05 FexOy = 94.61 FeO = 18.33 FexOy = 8.45CaO (%) 37.9 30.53 51.51 CaCO3 = 10 0.40 0.11MnO (%) 13.5 2.66 1.65 1.07 1.03MgO (%) 11.9 13.19 3.45 0.40 0.03Basicity: 2.49 1.73 3.81 – – – 2(CaO ? MgO)/ (Al2O3 ? SiO2)nr not reported Industrial Waste Aggregates
2.4 Industrial Slag 41Table 2.9 Mineralogical compositions of various slagsAuthors Country Type of slag Minerals identiﬁedRojas and Rojas Spain EAF-slag Wustite/plustite, magnesioferrite/magnetite, hematite, (2004) larnite, bredigite/merwinite, gehlenite, birnessite/groutellite (manganese oxides)Faraone et al. Italy EAF-slag Fine fraction: glaucochroite (CaMn)2SiO4, (2009) iron manganese oxide (FeMnO) Medium: calcite (CaCO3), glaucochroite (CaMn)2SiO4), iron manganese oxide (FeMnO), magnetite (Fe3O4), portlandite (Ca(OH)2)Tossavainen et al. Sweden LDF-slag Mayenite, (Ca12Al14O33), free MgO. b-Ca2SiO4, (2007) c-Ca2SiO4, Ca2Al2SiO7 BOF-slag Larnite, b-Ca2SiO4, solid solution of (Fe,Mg,Mn)O, solid solution of (CaMg)O EAF-slag, S1 Merwinite, Ca3Mg(SiO4)2, c-Ca2SiO4, solid solution of spinel phase (Mg, Mn)(Cr, Al)2O4 EAF-slag, S2 b-Ca2SiO4, wustite-type solid solution ((Fe, Mg, Mn)O), Ca2(Al, Fe)2O5, Fe2O3Qian et al. (2002) Singapore Kirschsteinite Kirschsteinite (CaFe2+(SiO4)), Mg-wustite based EAF- slagLuxan et al. (2000) Spain EAF-slag, S1 Major: gehlenite [Ca2 Al(Al,Si)2 O7], larnite (Ca2SiO4) and S2 Minor: bredigite [Ca14Mg2(SiO4)8], manganese oxides (Mn3O4, MnO2), magnesioferrite (MgFe2O4), magnetite (Fe3O4)while the granulated slag is used for cement manufacturing. Its use as aggregate inconcrete is not very usual although it has no behavioural problems, and there hasbeen little research work done on the subject. Because of their more porous structure, blast furnace slag aggregates havelower thermal conductivities than conventional aggregates. Their insulating valueis of particular advantage in applications such as frost tapers (transition treatmentsin pavement sub-grades between frost susceptible and non-frost susceptible soils)or pavement base courses over frost-susceptible soils. The granulated blast furnace slag is formed due to rapid quenching of moltenslag, which converts it into a glassy state. Granulated slag possesses cementitiousproperties if it is ground ﬁnely. The size and physical properties of granulated blastfurnace slag varies, depending on the chemical composition and method of pro-duction. Numerous studies are available on the properties of cement and concretecontaining ground blast furnace slag as a latent hydraulic material. Slag cement isthe hydraulic cement that results when molten slag from an iron blast furnace israpidly quenched with water, dried and ground to a ﬁne powder. Blast furnace slagsand was recognised as meeting JIS A 5012 standards in 1981, and has also beenstipulated in guidelines for the Japan Society of Civil Engineers. It is also stipu-lated as JIS A 5308 (ready-mixed concrete). Air-cooled blast furnace slag (air-cooled slag) is prepared by cooling the moltenblast furnace slag slowly by ambient air. A small amount of water is generally used
42 2 Industrial Waste Aggregatesto spray the surface of the slag to assist in the cooling process. The air-cooled blastfurnace slag is normally processed in a crushing and screening plant to manu-facture products of particular maximum sizes and gradings. Crushed air-cooledslag is angular, roughly cubical, and has textures ranging from rough, vesicularsurfaces to smooth glassy surfaces with conchoidal fractures. Processed air-cooledslag exhibits good abrasion resistance, good soundness characteristics and highbearing strength. The cementitious property of air-cooled slag is poorer than inother types of slag prepared by rapid quenching. Slag sand is very angular andcoarse and therefore mixes containing this product require a high ﬁne sand contentor the use of a mix containing three sand types. In general, blast furnace slagprocessed for use as a concrete aggregate complies with the same requirements fornaturally occurring dense aggregate. While complying with these requirements,air-cooled blast furnace slag aggregate differs from the range of naturally occur-ring dense aggregates in certain properties. The particle and bulk densities of air-cooled slag are slightly lower than those of natural aggregates. It has higher waterabsorption and Los Angeles value. Some typical properties of air-cooled slag arepresented in Table 2.10. If the molten slag is cooled and solidiﬁed by adding controlled quantities ofwater, air-, or steam, the resultant slag becomes a lightweight expanded or foamedtype of product. Foamed blast furnace slag is distinguishable from air-cooled slagby its relatively high porosity and low bulk density. Crushed expanded slag isangular, roughly cubical in shape and has a texture that is rougher than that of air-cooled slag. The porosity of expanded blast furnace slag aggregates is higher thanthat of air-cooled slag. The bulk relative density of expanded slag is difﬁcult todetermine accurately, but it is approximately 70 % of that of air-cooled slag.Typical compacted unit weights for expanded blast furnace slag aggregates rangefrom 800 to 1,040 kg/m3. The molten slag can be pelletised during cooling and solidiﬁcation process. Theproduced pellets can be made more crystalline or more vitriﬁed (glassy). Crys-talline pellet can be used as aggregate. The pelletised blast furnace slag has smoothtexture and round shape. Consequently, the porosity and water absorption aremuch lower than those of air-cooled or expanded slag. Pellet sizes range from 13to 0.1 mm, with the bulk of the product in the 1.0–9.5 mm range. Pelletised blastfurnace slag has a unit weight of about 840 kg/m3. Collins and Sanjayan (1999) reported the use of an air-cooled porous slag withmaximum diameter of 14 mm as a coarse aggregate in preparation of alkaliactivated slag concrete. The speciﬁc gravity of the slag aggregate was 2.71, whichwas slightly lower than used basalt aggregate (2.95). The water absorptioncapacity of slag was 4.4 % and considerably higher than basalt aggregate (1.2 %). Etxeberria et al. (2010) reported the use of blast furnace slag of size range of4.75–25 mm as a complete or partial replacement of coarse aggregate in prepa-ration of concrete. The physical properties of the aggregate were determinedaccording to British standard, BS EN 1097-6:2000. The oven dry and saturatedsurface dry densities of the aggregate were 2.27 and 2.37 g/cm3 respectively ,which are lower than the used natural aggregate (about 2.7 g/cm3). On the other
2.4 Industrial Slag 43Table 2.10 Typical mechanical properties of air-cooled blast furnace slag (FHWA-RD-97-148)Property ValueLos Angeles abrasion (ASTM C131) 35–45 %Sodium sulphate soundness loss (ASTM C88) 12 %Angle of internal friction 40–45Hardness (measured by Mohr’s scale of mineral hardness)a 5–6California bearing ratio (CBR), top size 19 mm (3/4 in)b up to 250 %a Hardness of dolomite measured on same scale is 3–4b Typical CBR value for crushed limestone is 100 %hand, the water absorption capacity of slag aggregate was 4.10 % and lower thanthat of natural aggregate (2.94 %). Yuksel et al. (2011) used granulated blast furnace slag (GBFS) with maximumdiameter of 4 mm as partial replacement of ﬁne aggregate in concrete. The variousproperties of GBFS aggregate along with a natural ﬁne aggregate are presented inTable 2.11. Escalante-García et al. (2009) reported the use of a GBFS as ﬁne aggregate incement mortar. The GBFS employed as an aggregate was used as received andonly a fraction of large sized particles was removed; 90 % was retained in the0.420 mm sieve and 28 % was retained in the 1 mm sieve. The used GBFS hassharp edges and some particles have several surface pores. Leshchinsky (2004) reported the use of air-cooled slag sand with maximum sizeof 6.3 mm as a ﬁne aggregate in ready-mixed concrete. The moisture content ofthe used slag sand is within a range of 2–4 % above the saturated surface dry(SSD) content. According to the author, complete saturation is crucial for slagaggregate and for slag sand to achieve the required concrete properties.2.4.2 Non-Ferrous SlagNon-ferrous metallurgical slags are generated during reﬁning of various metalssuch as Cu, Cr, Zn and treatment of waste such as Pb-acid batteries. Some physicalproperties of a few non-ferrous slags are presented in Table 220.127.116.11.2.1 Copper SlagCopper slag is a by-product obtained during the matte (molten copper sulphide)smelting and reﬁning of copper (Biswas and Davenport 1976). Major constituentsof a smelting charge are sulphides and oxides of iron and copper. The charge alsocontains oxides such as Al2O3, CaO, MgO, and principally SiO2, which are eitherpresent in the original concentrate or added as a ﬂux. As a result, copper-rich matte(sulphides) and copper slag (oxides) are formed as two separate liquid phases. The
44 2 Industrial Waste AggregatesTable 2.11 Physical properties of granulated blast furnace slag (Yuksel et al. 2011)Property Type of aggregate GBFS NaturalLoose bulk density (kg/m3) 1,052 1,930Dense bulk density (kg/m3) 1,236 1,950Speciﬁc gravity 2.08 2.60Water absorption (%) 8.30 2.30Amount of clay (%) 1.0 4.0Loss on ignition (%) 1.8 5.0Lightweight particles (%) 3.0 4.0Table 2.12 Some physical properties of various non-ferrous slags (Publication number: FHWA-RD-97-148)Property Nickel slag Copper slag Phosphorus slag Lead, lead–zinc, and zinc slagsAppearance Reddish brown to Black Black to dark grey Black to red brown-blackTexture Massive, angular, Glassy, more Air-cooled is ﬂat and Glassy, sharp amorphous vesicular elongated but granulated angular texture when is uniform, angular (cubical) granulated particlesUnit weight, 3,500 2,800–3,800 Air-cooled: 1,360–1,440 2,500–3,600 (kg/m3) Expanded: 880–100Absorption (%) 0.37 0.13 1.0–1.5 5.0molten slag is discharged from the furnace at 1,000–1,300 °C. When liquid slag iscooled slowly, it forms a dense, hard crystalline product where a quick solidiﬁ-cation by pouring molten slag into water provides amorphous granulated slag.Production of one tonne of copper generates approximately 2.2–3 tonnes of copperslag. In the United States the amount of copper slag produced is about four milliontonnes (Collins and Ciesielski 1994), in Japan it is about two million tonnes peryear (Ayano and Sakata 2000), and approximately 360,000, 244,000 and60,000 tonnes of copper slag are produced every year in Iran, Brazil and Oman,respectively (Behnood 2005; Moura et al. 1999; Taeb and Faghihi 2002). Recycling, recovering of metal, production of value added products anddisposal in slag dumps or stockpiles are the options for management of copperslag. It has been widely used for abrasive tools, rooﬁng granules, cutting tools,abrasive, tiles, glass, road-base construction, railroad ballast, asphalt pavements,cement clinker and blended cement production (Shi et al. 2008). Many researchershave investigated the use of copper slag as ﬁne or coarse aggregate in the prep-aration of cement mortar and concrete. The main concern in large-scale use of copper slags including in construction isthe content of toxic elements in copper slag and the consequent leaching from slagand slag based products. However, copper slag has been excluded from the listedhazardous waste category of the United States Environmental Protection Agency
2.4 Industrial Slag 45(USEPA). The United Nations (UN) Basel Convention on the TransboundaryMovement of Hazardous Waste and its Disposal also ruled that copper slag is not ahazardous waste (Alter 2005). The chemical composition of copper slag depends on the type of furnace, themetallurgical production process, and the composition of the extracted ore. Therange of percentage of the main oxides of copper slag can vary as follows—Fe2O3:35–60 %, SiO2: 25–40 %, CaO: 2–10 %, Al2O3: 3–15 %, CuO: 0.3–2.1 %, MgO:0.7–3.5 %. The density of copper slag varies between 3.16 and 3.87 g/cm3, theaverage speciﬁc gravity of copper slag is about 3.5 g/cm3 and the average waterabsorption of copper slag is 0.15–0.55. Water-cooled copper slag has a higherwater absorption and lower unit weight than air-cooled copper slag due to its moreporous texture (Shi et al. 2008). Air-cooled copper slag has a black colour andglassy appearance. The speciﬁc gravity varies with iron content, from 2.8 to 3.8.The unit weight of copper slag is somewhat higher than that of conventionalaggregates. The absorption capacity of the material is typically very low (0.13 %).Granulated copper slag is more porous and therefore has lower speciﬁc gravity andhigher absorption capacity than air-cooled copper slag. The granulated copper slagis made up of regularly shaped, angular particles, mostly between 4.75 and0.075 mm in size (Emery 1995; Hughes and Halliburton 1973). Air-cooled and granulated copper slag has a number of favourable mechanicalproperties for aggregate use, including excellent soundness characteristics, goodabrasion resistance, and good stability. It has high friction angle due to sharp angularshape. However, the slag tends to be vitreous or ‘glassy,’ which adversely affects theirfrictional properties (skid resistance), a potential problem if used in pavement surfaces. Khanzadi and Behnood (2009) reported the use of copper slag as a coarseaggregate in concrete, which meet the grading requirements of ASTM C 33 for12.5–4.75 mm size aggregates. The physical properties of the copper slag aggre-gates along with a coarse natural limestone aggregate are presented in Table 2.13.The used copper slag has signiﬁcantly higher speciﬁc gravity than the limestoneaggregate. The high speciﬁc gravity and the glass-like smooth surface properties ofirregular grain shape of copper slag aggregates can increase bleeding. The waterabsorption capacity of copper-slag is 0.4 % and lower than limestone aggregate,which is 0.6 %. Copper slag aggregate is harder than natural limestone aggregate. Wu et al.(2009) reported the use of copper slag as a ﬁne aggregate in concrete.The copper slag used in this investigation had a density of 3,660 kg/m3, in contrastwith the density of sand of 2,640 kg/m3. The ﬁneness modulus of the copper slagwas 1.78, which was ﬁner than sand, with a ﬁneness modulus of 2.91. The particlesize of the copper slag was well distributed within the range of 0.1–1 mm. Theshape of sand is irregular with rounded edges at 50 9 magniﬁcation while that ofcopper slag is angular with sharp edges. The surface texture of sand is rougher thanthat of copper slag at 200 9 magniﬁcation. Under observation at 1,000 9 mag-niﬁcation the presence of moisture on sand surface is visible, but the surface ofcopper slag is glassy and dry. Al-Jabri et al. (2011) reported the use of a copper slag as a ﬁne aggregate in thepreparation of cement mortar and concrete. Before using the slag, the material was
46 2 Industrial Waste AggregatesTable 2.13 Some physical properties of copper slag and limestone aggregate (Khanzadi andBehnood 2009)Properties Copper slag aggregate Limestone aggregateSpeciﬁc gravity, g/cm3 3.59 2.65Aggregate crushing value, % 10–21 23Aggregate impact value, % 8.2–16 11Water absorption, % 0.4 0.6Particle size, mm 4.75–12.5 4.75–12.5grinded in the laboratory into a ﬁne powder to the required size. The particle sizedistribution of the ground slag along with normal sand is presented in Fig. 2.6. Copper slag has high concentrations of silica, alumina and iron oxides. Resultsfrom speciﬁc gravity and water absorption tests revealed that copper slag has aspeciﬁc gravity of 3.4 which is higher than that of sand (2.77), whereas the waterabsorption values for copper slag and sand were about 0.2 and 1.4 %, respectively. Brinda et al. (2010) used a copper slag as partial replacement of sand andcement in concrete preparation. The physical properties of copper slag are pre-sented in Table 2.14. The slag was made of black glassy particles and granular innature and has a particle size range similar to sand. The speciﬁc gravity of the slagis 3.91. The bulk density of granulated copper slag varied from 1.9 to 2.15 kg/m3,which is almost similar to the bulk density of conventional ﬁne aggregate. Thehardness of the slag lies between 6 and 7 in the Mohr scale. This is almost equal tothe hardness of gypsum. The pH of aqueous solution of aqueous extract as per IS11127 varies from 6.6 to 7.2. The free moisture content present in slag was foundto be less than 0.5 %. The amount of silica in slag is about 26 %. The ﬁneness ofcopper slag was calculated as 125 m2/kg. Ishimaru et al. (2005) reported the use of a copper slag as a replacement of sandin the preparation of concrete. The density, water absorption and ﬁneness modulusof used copper slag are respectively 3.46 g/cm3, 0.65 and 2.58 %.18.104.22.168 Other Non-ferrous SlagsThe use of other non-ferrous industrial slags as aggregate in concrete and cementmortar is also reported. Lead slag generated from lead smelting and from recyclingof secondary lead batteries may be used as ﬁne and coarse aggregate in thepreparation of cement mortar and concrete. Atzeni et al. (1996) reported the use of granulated slag generated duringsmelting of lead and zinc by two different processes (named as Imperial Smeltingand Kivcet slags), as a partial and total replacement of the sand fraction in cementmortar and concrete. The slags were used as received from granulation plants.Both types of slags were essentially vitreous with small amount of gehlinite,crystobalite and iron oxides as minor crystalline components. Both slags containFeO, SiO2, CaO and Al2O3 as the major oxides with signiﬁcant amounts of zinc
2.4 Industrial Slag 47Fig. 2.6 Sieve analysis of atypical copper slag alongwith normal sand aggregate(Al-Jabori et al. 2011)Table 2.14 Some physical Particle shape Irregularproperties of copper slag(Brinda et al. 2010) Appearance Black and glassy Speciﬁc gravity 3.91 Percentage of voids 43.20 % Bulk density 2.08 g/cm3 Fineness modulus 3.47 Angle of internal friction 51°200and lead. Most slag grains are rounded and others are polygonal as a result ofconchoidal fracture caused by thermal shock induced by granulation. ImperialSmelting slag is generally less regular than Kivcet slag. The grain size distributionof both slags is similar to that of normal sand. The predominant fraction by mass isthe 0.15–2 mm size range. The grains have very low porosity, on average 1 % byvolume for the K slag and 3 % by volume for the IS slag. Penpolcharoen (2005) reported the use of a secondary lead slag as an admixtureand/or as an aggregate in the production of concrete blocks. The slag was producedfrom battery smelting using CaCO3 as ﬂux. The ﬁne fraction of slag, which passedthrough ASTM sieve No. 200, was used as a partial substituent of ordinaryPortland cement, while the coarse fraction of slag, which passed through ASTMsieve No. 4, was used to partially replace crushed limestone aggregate. The CaOcontent in slag is 6.2 times less than that in OPC, whereas its iron content, as FeO,is 15.1 times higher. The Fe in slag is mainly contained as FeO and thereforeweight gain was observed during determination of loss on ignition test. Thephysical properties of ﬁne and coarse fractions of slags are presented in Table 2.15along with OPC and crushed stone aggregate. Sorlini et al. (2004) reported the use of two different types of slag that containedvery high amounts of Zn as aggregate in the preparation of concrete. A fresh slagobtained after water cooling and a cured slag after storage of about 6 months inlandﬁll were used in this study. The slag is generated as a by-product of theconversion of electric arc furnace (EAF) dusts (with zinc concentration of18–35 %) into an impure zinc oxide, called Waelz oxide (with zinc concentration
48 2 Industrial Waste AggregatesTable 2.15 Some physical properties of secondary lead slag (Penpolcharoen 2005)Property OPC Fine slag Crushed stone Coarse slagSpeciﬁc gravity 3.15 3.62 2.71 3.62Blain ﬁneness 3,380 3,333 – –Fineness modulus – – 4.74 4.70of 55–65 %), that can be reprocessed in metallurgical plants. This slag is classiﬁedas dangerous waste. Both slags contain very high concentrations of calcium(43 %). Zinc and lead concentrations are about 6 and 1 % respectively; othermetals, like manganese, cadmium, copper, chromium and arsenic, are also presentin considerable amounts. However, the leachability of these toxic elements inconcrete blocks with this slag as aggregate is within the speciﬁed limit. Zelic (2005) investigated the use of a high-carbon ferrochromium slag asaggregate in the preparation of concrete. Before using the slag as aggregate, theoriginal air-cooled slag was crushed to a grain size in the range of 0–16 mm, ﬁrstby a hammer crusher and then by a cone beaker. The metallic globules of ferro-chromium metal were then removed from the crushed slag by the Remer jigtreatment by means of difference in speciﬁc gravities of slag and metallic fraction.The speciﬁc gravity of slag and FeCr metal is 3.2 and 7.1 g/cm3, respectively. Thereﬁned slag (0–16 mm) fraction contains up to the 11 % Cr. The part of the Cr2O3 component in the slag is 8.3 % in mass smaller after thejig treatment than in the original slag before the treatment, which was the actualaim of the applied process of metal concentration and its removal from the slag.No chlorides were observed in the slag and the sulphur SO3 content of 0.50 % inmass is much lower than the allowed value of 1.00 % in mass, indicating that theslag does not contain harmful components that may be found in aggregates. Themajor minerals present in slag are: forsterite, (Mg, Fe)2SiO4, common-spinel(MgAl2O4), chrome-spinel ((Mg, Fe)(Cr,Al)2O4) as unaltered chromium ore andalso of small amounts of enstatite (MgSiO3). The slag exhibits better performancethan normal limestone aggregate during the Loss Angeles and Bohme wear tests.The ﬁneness modulus of the unfractionated slag varied from 4.0 to 5.1 suggesting atoo uneven size distribution of the slag, as the upper acceptable limit is 3.6. Thevolume mass of ferrochromium slag particles is about 3,250–3,310 kg/m3 and thatof the limestone ones about 2,700 kg/m3. The Faury coefﬁcients, k, obtained forboth the (4–8 mm) and the (8–16 mm) fractions of slag are 0.17 and 0.22,respectively. The results of the mortar bar expansion test indicate the slagaggregate as non-reactive in terms of alkali-silica reaction. The frost resistance ofslag is comparable to natural limestone aggregate and well within the standardspeciﬁcations. Morrison et al. (2003) reported the use of ferro-silicate slag, generated duringthe production of zinc in Imperial Smelting Furnace (ISF-slag) was as aggregate inconcrete road construction (Morrison et al. 2003, Morrison and Richardson 2004).The slag is glassy and granular in nature and has a particle size range similar tosand, indicating that it could be used as a replacement for sand present in
2.4 Industrial Slag 49cementitious mixes. The density of this slag (3,900 kg/m3) is higher than that oftraditional aggregates, suggesting it may have advantages over these aggregatematerials in certain applications, such as in noise barriers. The X-ray diffraction(XRD) showed the presence of inclusions of metallic iron, although the principalcrystalline components detected were FeO and ZnS. Metwally et al. (2005) reported the use of a slag produced from recycling ofspent lead-batteries as aggregate in concrete production. Recycled-lead slag (RLS)was used as both ﬁne and coarse aggregate in concrete manufacture after crushinginto the desired gradation by using a roller mill. The physical and mechanicalproperties of the used ﬁne aggregate (sand and ﬁne lead-slag) and coarse aggregate(gravel and coarse lead-slag) are given in Table 2.16. The coarse lead-slag werewashed carefully and dried before mixing to remove any impurities and organicmatters, which may weaken its bond with the cement paste. Mixing water wasclean tap water free from impurities and organic matters. Pereira et al. (2000) reported the use of a salt cake slag, produced from alu-minium scrap re-melted as partial replacements of either sand or cement in thepreparation of cement mortar production after washing. Non-washed slags cannotbe mixed with cement due to the volumetric expansion observed during setting,high chloride content and release of high concentrations of noxious gases. As theconcentrations of some toxic elements in the majority of these slags are very high,before application the environmental suitability as well as the long-termmechanical and durability performance of concrete containing slag must beevaluated for the application of these materials as aggregate in concrete.2.5 Other Waste as AggregateThe meat and bone mill bottom ash (MBM-BA) used by Cyr and Ludmann (2006) asa ﬁne aggregate in cement mortar preparation has a grading size between 0 and 2 mmand a mean diameter of 0.4 mm (Fig. 2.7). The physical properties of MBM-BA arepresented in Table 2.17. The bulk density of MBM-BA is around 900 kg/m3 andmuch lower than that of normal sand (1,500 kg/m3). The average density of the ash is2,900 kg/m3. The external speciﬁc surface area, calculated from the density and theparticle size distribution (considering cylindrical particles), is about 3 m2/g. TheBET method gives a speciﬁc surface area of 3,000 m2/kg, which is a thousand timeshigher than the value calculated using the particle size distribution. This signiﬁcantdifference is related to a large open porosity of the grains, leading to water absorptionof 11 %, a very high value compared to normalised siliceous sand (less than 1 %). The strength of MBM-BA is evaluated using a friability coefﬁcient, deﬁned asthe ratio between the mass of crushed particles (less than 0.1 mm) and the wholemass of material before crushing. The friability coefﬁcient of MBM-BA, measuredas 37 %, is well within the speciﬁed value, which is 40 % for 60 MPa concreteintended for building construction.
50 2 Industrial Waste AggregatesTable 2.16 Physical properties of ﬁne and coarse lead slags along with natural aggregates(Metwally et al. 2005)Property Natural sand Natural gravel Fine lead slag Coarse lead slagSpeciﬁc gravity 2.57 2.51 4.28 3.79Density (kg/m3)Loose 1,600 1,530 2,280 1,990Dense 1,869 1,640 2,820 2,120Voids (%)Loose 38 39 47 47Dense 27 35 34 44Water absorption (%) 0.42 0.35 3.95 2.35Fineness modulus 2.49 6.90 3.35 6.95Crushing value (%) – 13.5 – 29.3Impact value (%) – 6.82 – 13.4Loss Angeles value (%) – 16.7 – 47.0 The major minerals present in MBM-BA are hydroxylapatite Ca5(PO4)3(OH)and whitlockite Ca3(PO4)2. Calcium hydroxylapatite is the major inorganic con-stituent of bones and teeth. Trace amounts of some minerals such as quartz,hematite and magnetite are also present in MBM-BA, which probably came fromother waste used as co-combustion materials. Although MBM-BA contains smallamounts of trace elements, the leachability of these meets the regulation set byFrench Government for using in road construction. Öztürk and Bayrakl (2005) investigated the possibilities of the use of tobacco waste,a by-product in a cigarette factory as aggregate in lightweight concrete production.The organic and water content in this aggregate are 66.21 and 25.45 % respectively. Yellishetty et al. (2008) evaluated the recycling potential of four different ironore mineral wastes as aggregate in the preparation of concrete. The waste wascollected randomly, from different fresh waste dumps as recommended ASTMD75; C702 sampling of aggregates. It was mixed to form a representativehomogeneous mixture. The sieve analyses of typical particle overburden materialfrom the waste dumps of the corresponding iron ore mines are presented inFig. 2.8. A volume equivalent of approximately 50 % of the total is within theusable range as aggregates for making of concrete cubes. Of the whole volume,20 % is in the range of sand–silt–clay material. Variability in size distribution is anindication of inherent geological properties of mine waste material and of thecrushing and compaction that waste undergoes while breaking/loosening. Various physico-mechanical properties of the mine waste were measuredaccording to ASTM methods and presented in Table 2.18. In aggregates fromdifferent mines, the ﬁneness modulus (FM) was within the range of IS2386speciﬁcations prescribed for aggregate for civil constructions. Most of the physicalproperties of the mine aggregates, belonging to different mines, were within ±5 %range of standard speciﬁcations and were in conformity with the concurrent IndianStandards for aggregates.
2.5 Other Waste as Aggregate 51Fig. 2.7 Particle sizedistribution of MBM-BA, incomparison with the limitsfor sand used for standardmortar (Cyr and Ludmann2006)Table 2.17 Physical Density (kg/m3) 2,900properties of meat and bone 3mill ash (Cyr and Ludmann Bulk density (kg/m ) 9002006) Speciﬁc surface area, BET (m2/kg) 3,000 Particle size range (mm) 0–2 Mean diameter (mm) 0.4 Morphology Irregular particles Adsorption coefﬁcient (water) (%) 11 Friability coefﬁcient (%) 37 Gallardo and Adajar (2006) reported the use of paper mill sludge as a partialreplacement of ﬁne aggregate in concrete preparation. The composition of papersludge is generally a function of the raw material, manufacturing process, chem-icals used, ﬁnal products and wastewater treatment techniques. Sludge from pulpand paper mills are mainly cellulose ﬁbres generated at the end of the pulpingprocess prior to entering the paper machines. Paper sludge obtained directly from amill wastewater treatment plant is composed generally of 50–75 % organics(cellulose ﬁbres and tissues) and 30–50 % kaolinite clay. The paper mill sludgeused in this study was air-dried for several days and facilitated by an artiﬁcialmethod using a blow drier. The dry sludge was then crushed and sieved using sieveNo. 4 to separate the ﬁne particles to be used as ﬁne aggregates in the mix. Thephysical properties of paper sludge along with ﬁne aggregates (sand) are presentedin Table 2.19. Sludge was lighter than normal sand and it has very high waterabsorption capacity. The large absorption percentage of sludge is indicative of itshigh porosity or entrapped air content and that it absorbs water faster than sand.The high absorption rate is due to hydrogen bonding in the property of sludge.There was no silica content in paper sludge while calcium and iron is of lesseramount as compared to ﬁne aggregates. Some other element contents in papersludge are lower than the normal sand. Ahmadi and Al-Khaja (2001) investigated the use of paper sludge, obtained froma tissue paper manufacturing facility as partial replacement of ﬁne aggregate in thepreparation of concrete. The sieve analysis of sludge and normal sea sand indicates
52 2 Industrial Waste AggregatesFig. 2.8 Sieve analysis ofmine wastes (Yellishettyet al. 2008)that the used sludge is coarser than the sea sand. About 50 % of the particles ofsludge are coarser than 2 mm compared with sea sand in which 100 % of theparticles pass the 2.36 mm sieve. The chemical analysis of the waste shows that ithas a low pH value with acceptable levels of other chemical parameters and fallswithin the permissible limits established in Bahrain for use of waste in construction. Kuo et al. (2007) reported the use of petroleum reservoir sludge as ﬁneaggregate in the preparation of cement mortar. The composition of sludge ispresented in Table 2.20. The sludge contains very high amount of smectite clay([60 %), which can cause a detrimental expansion to some extent, when it ismixed with water. Hence, reservoir sludge cannot be directly used as ﬁne aggre-gates in concrete and therefore, before using it as aggregate, hydrophilic sludge isconverted into hydrophobic by using a cationic surfactant. The sieve analysis of modiﬁed sludge organically modiﬁed reservoir sludge(OMRS) along with normal sand is presented in Table 2.21. More than 80 % ofthe OMRS particles are smaller than 0.6 mm but larger than 0.075 mm. From thethermal analysis of reservoir sludge before and after the treatment, the authorsconﬁrmed that the OMRS particles have been organically modiﬁed and becamehydrophobic before they were mixed with water, quartz sands and cement. Kinuthia et al. (2009) reported the use of dark coloured colliery spoil, generatedduring mining of coal as replacement of ﬁne and coarse aggregate in the prepa-ration of medium strength concrete. It was obtained as two materials, a ﬁnefraction of low plasticity, and a coarser non-plastic fraction. The two fractionswere blended in equal proportions to produce a well-graded colliery spoil material,which is presented in Fig. 2.9 along with other constituents of prepared concrete.The speciﬁc gravity of both types of spoils was 1.8 and lighter than normalaggregate. Ilangovana et al. (2008) reported the use of quarry rock dust as ﬁne aggregate inthe preparation of concrete. The authors deﬁned the quarry rock dust as residue,tailing or other non-valuable waste material after the extraction and processing ofrocks to form ﬁne particles less than 4.75 mm. The level of utilisation of this dust innations like Australia, France, Germany and UK has reached more than 60 % of itstotal production. The physical properties of the used dust are presented in Table 2.22.
2.5 Other Waste as Aggregate 53Table 2.18 Physical properties of various mine waste aggregates (Yellishetty et al. 2008)Properties Sample 1 Sample 2 Sample 3 Sample 4Fineness modulus: coarse 7.5 8.0 7.0 8.0Fineness modulus: ﬁne 3.3 3.4 3.2 3.5Flakiness index, % 10 13 14 11Elongation index, % 11 15 14 11Impact value, % 19.09 29.00 15.75 21.94Speciﬁc gravity 2.5 2.3 2.6 2.5Water absorption, % 11.00 13.10 5.59 8.13Bulk density: rodded, kg/l 1.39 1.25 1.40 1.30Bulk density: loose, kg/l 1.36 1.22 1.30 1.20Void ratio: rodded, % 44.40 46.80 46.00 48.00Void ratio: loose, % 45.60 48.08 47.00 52.00Crushed value, % 30.0 30.0 28.6 29.9Abrasion value, % 29.42 30.00 30.00 29.00Angularity number 3 3 1 7Table 2.19 Properties of Properties Sand Sludgenormal sand and paper sludge(Gallardo and Adajar 2006) Moisture content (%) 10.00 25.77 Speciﬁc gravity 2.60 1.57 Water absorption (%) 4.00 22.35 Silica (%) 18.91 0.00 The major oxide composition of the quarry rock dust and ﬁne sand is presentedin Table 2.23. Rock dust contains lesser amounts of silica and higher amounts ofalumina, iron oxide, calcium oxide, magnesium oxide and titanium oxide thannatural sand. On the other hand, the total alkali content in these materials is almostthe same.2.6 Ceramic Industry WasteIn the ceramic industry several types of waste are generated. According toPacheco-Torgal and Jalali (2010), ceramic waste can be separated into two cate-gories in accordance with the source of raw materials. In each category, the ﬁredceramic waste was classiﬁed according to the production process. This classiﬁ-cation is presented in Fig. 2.10. These were produced by using red and whiteceramic pastes. However, the use of white paste is more frequent and much higherin volume. It has been estimated that about 30 % of the daily production in the ceramicindustry goes to waste (Senthamarai and Devadas 2005). In Europe, the amount ofwaste in the different production stages of the ceramic industry reaches 3–7 % of
54 2 Industrial Waste AggregatesTable 2.20 Composition of reservoir sludge (Kuo et al. 2007)Physical propertiesGravel content, % 0Sand content % 0Silt content 31.9Clay content 68.1Speciﬁc gravity 2.72Chemical compositionSilica 53.03Alumina 22.32Iron oxide 8.56Others 16.09Table 2.21 Sieve analysis of sludge (OMRS) and quartz sands (Kuo et al. 2007)OMRS Quartz sandSieve size Cumulative passing (%) Sieve size Cumulative passing (%)4.75 100 4.75 1002.36 100 2.36 1001.18 100 1.18 98.60.600 100 0.600 26.20.300 86.8 0.300 3.40.150 55.2 0.150 1.40.075 19.3 0.075 0.2Fig. 2.9 Particle size distributions of colliery waste along with other materials (Kinuthia et al.2009)its global production (Fernandes et al. 2004). Although the reutilisation of ceramicwaste has been practiced, the amount of waste reused in that way is still negligible(Pacheco-Torgal and Jalali 2010). Ceramic waste can be used safely in the pro-duction of concrete due to some of its favourable properties. Ceramic waste isdurable, hard and highly resistant to biological, chemical and physical degradation
2.6 Ceramic Industry Waste 55Table 2.22 Physical properties of quarry rock dust and natural sand (Ilangovana et al. 2008)Properties Quarry rock dust Fine sandSpeciﬁc gravity 2.54–2.60 2.60Bulk relative density (kg/m3) 1,720–1,810 1,460Water absorption (%) 1.2–1.5 NilMoisture content (%) Nil 1.5Particles ﬁner than 0.075 mm (%) 12–15 6Sieve analysis (Indian standard speciﬁcation) Zone II Zone IITable 2.23 Oxide Oxide constituents Quarry rock dust (%) Natural sand (%)composition of quarry rockdust and natural sand SiO2 62.48 80.78(Ilangovana et al. 2008) Al2O3 18.72 10.52 Fe2O3 6.54 1.75 CaO 4.83 3.21 MgO 2.56 0.77 Na2O Nil 1.37 K2O 3.18 1.23 TiO2 1.21 Nil Loss on ignition 0.48 0.37forces. In the following paragraphs, the aggregate properties of some ceramicwaste will be discussed. The waste used by Senthamarai and Devadas (2005) as coarse aggregate in thepreparation of normal concrete was collected from a ceramic electrical insulatorindustry. The material was too big to be fed into a crushing machine and thereforeit was broken into small pieces of about 100–150 mm with a hammer. The surfacewas also deglazed manually by chisel and hammer. These small pieces were thenfed into a jaw crusher to reach the required 20 mm size. The various physical properties of waste as well as those of natural aggregatesare presented in Table 2.24. According to the same authors, the properties ofceramic waste aggregate were similar to those of natural crushed stone aggregate.The speciﬁc gravity and ﬁneness modulus of aggregate were 2.45 and 6.88respectively. The surface texture of the ceramic waste aggregate was found to besmoother than that of crushed stone aggregate. In the soundness test, after 30 cycles,the weight loss of ceramic waste aggregate was 51 % less than that of conventionalcrushed stone aggregate, since ceramics are more resistant to all chemicals. Binici (2007) used ceramic industry waste as a partial replacement of ﬁneaggregate (40–60 %) in the preparation of normal concrete. The bigger wastepieces were processed into the 4 mm or less size range by a procedure similar tothat adopted by Senthamarai and Devadas (2005). The size grading of the wasteceramic ﬁne aggregate was suitable for concrete production. The various physicalproperties of the waste aggregate are given in Table 2.25 along with those ofconventional ﬁne aggregate. Like the coarse aggregate properties of ceramic waste
56 2 Industrial Waste AggregatesFig. 2.10 Classiﬁcation of ceramic wastes according to Pacheco-Torgal and Jalali (2010)reported by Senthamarai and Devadas (2005), the properties of ﬁne waste aggre-gates are similar to those of ﬁne conventional aggregate. Chemically the ceramicwaste ﬁne aggregate is composed of silica (88.4 %) with 7.3 % of aluminium oxide. Suzuki et al. (2009) used a porous waste ceramic coarse aggregate in thepreparation of high-performance concrete. The aggregate was recovered from thewaste of a local ceramic production plant. The aggregate was used in saturatedsurface-dry conditions. Table 2.26 summarises the main characteristics of the porous ceramic wasteaggregate along with natural coarse and ﬁne aggregates and a commercial light-weight coarse aggregate that is used for internal wet-curing purposes. The particles of the waste ceramic aggregate are coarser than those of thenatural coarse aggregate (Fig. 2.11). Topcu and Canbaz (2007) reported the use of crushed tile waste as aggregate inthe preparation of concrete. Tile is produced from natural materials sintered at hightemperatures and it does not contain any harmful chemicals. The tile waste wascrushed into 4–16 mm and 16–31.5 mm sizes before using. The unit weight,speciﬁc weight and water absorption of crushed tiles were 925, 1,904 kg/m3 and11.56 % respectively. Abrasion losses were 21 and 82 % for the Los Angelesabrasion tests at 100 and 500 cycles, respectively. The abrasion of crushed tile wasquite high. The maximum amount of abrasion was 50 % at 500 cycles. Guerra et al. (2009) investigated the use of a crushed recycled sanitary porcelainceramic ranging from 5 to 20 mm as a partial substitution of natural coarse aggregate.The composition of the clay from which sanitary porcelain was made was: quartz30 %, feldspar 26 %, kaolin 26 %, clay 18 % and lastly, glazes and metal oxides.The waste was used without cleaning due to the purity of the materials. However,the porcelain was crushed and sieved in the laboratory to get the required size range.The density and moisture content in the porcelain aggregate were 2.36 g/cm3 and